The influence of ligand configuration, solvent size and solvent polarity on the porous shape and void volume in a series of isomeric or isomorphic porous MOFs
Huang, Wen-Huan; Luan, Xin-Jun; Zhou, Xiang; Chen, Jun; Wang, Yao-Yu; Shi, Qi-Zhen; CrystEngComm 15 (2013) 10389–; doi:10.1039/c3ce41801d

data_7214607
_publ_section_title
;
 The influence of ligand configuration, solvent size and solvent polarity
 on the porous shape and void volume in a series of isomeric or isomorphic
 porous MOFs
;
_journal_issue                   47
_journal_name_full               CrystEngComm
_journal_page_first              10389
_journal_paper_doi               10.1039/c3ce41801d
_journal_volume                  15
_journal_year                    2013
_chemical_formula_sum            'C192 H Mn12 N8 O88'
_chemical_formula_weight         4486.29
_chemical_name_systematic
;
?
;
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 97.507(2)
_cell_angle_gamma                90.00
_cell_formula_units_Z            1
_cell_length_a                   12.5497(12)
_cell_length_b                   21.783(2)
_cell_length_c                   17.7472(16)
_cell_measurement_temperature    293(2)
_cell_volume                     4810.0(8)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.956
_diffrn_measured_fraction_theta_max 0.956
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1181
_diffrn_reflns_av_sigmaI/netI    0.2103
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       29
_diffrn_reflns_limit_k_min       -26
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            29376
_diffrn_reflns_theta_full        28.70
_diffrn_reflns_theta_max         28.70
_diffrn_reflns_theta_min         1.49
_exptl_absorpt_coefficient_mu    0.862
_exptl_absorpt_correction_T_max  0.8362
_exptl_absorpt_correction_T_min  0.7474
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   sadabs
_exptl_crystal_density_diffrn    1.549
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             2213
_exptl_crystal_size_max          0.32
_exptl_crystal_size_mid          0.27
_exptl_crystal_size_min          0.19
_refine_diff_density_max         0.656
_refine_diff_density_min         -0.748
_refine_diff_density_rms         0.140
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.002
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     684
_refine_ls_number_reflns         11870
_refine_ls_number_restraints     6
_refine_ls_restrained_S_all      1.002
_refine_ls_R_factor_all          0.2123
_refine_ls_R_factor_gt           0.0692
_refine_ls_shift/su_max          0.036
_refine_ls_shift/su_mean         0.003
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0830P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1491
_refine_ls_wR_factor_ref         0.2293
_reflns_number_gt                4504
_reflns_number_total             11870
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c3ce41801d.txt
_cod_data_source_block           xb5543_0m
_cod_original_sg_symbol_H-M      P21/c
_cod_database_code               7214607